A PROTOCOL FOR DETERMINATION OF THE ADHESIVE FRACTURE TOUGHNESS OF FLEXIBLE LAMINATES BY PEEL TESTING: FIXED ARM AND TPEEL METHODS


 Mavis Chapman
 1 years ago
 Views:
Transcription
1 1 A PROTOCOL FOR DETERMINATION OF THE ADHESIVE FRACTURE TOUGHNESS OF FLEXIBLE LAMINATES BY PEEL TESTING: FIXED ARM AND TPEEL METHODS An ESIS Protocol Revised June 2007, Nov 2010 D R Moore, J G Williams 1 INTRODUCTION. Flexible laminates are used in a wide range of industrial and packaging applications. In general, there will be considerable practical importance associated with the adhesive strength between adjacent laers in these laminates. Sometimes it will be important to maximise this adhesive strength, sometimes it will be required to minimise it. Overall, the ke requirement will be to control it and to achieve this it is first necessar to measure it. The purpose of this protocol is to provide guidance on the measurement of peel strength of the laminate and then to show how the adhesive fracture toughness (also known as adhesive strength or interfacial work of fracture can be determined from this peel strength and other measurements. Other standards provide guidance on conducting peel tests on flexible laminates (eg ISO and ISO Peel test for a flexiblebondedtorigid specimen assembl, Part 1 90 o peel and Part o peel. ISO o peel test for flexibletoflexible bonded assemblies (Tpeel test. These procedures indicate how to measure peel strength (force per unit width for peeling but do not include additional test information and analsis for converting peel strength to adhesive fracture toughness. There are important distinctions between these two properties in that peel strength indicates how difficult it is to peel one substrate from another, but adhesive fracture toughness is indicative of how well the two substrates are stuck together. It is this latter propert that is most often sought. The protocol is divided into two parts; one for a fixed arm peel test and the other for a Tpeel test. These geometries are different but there is a common aim in converting the peel strength measurement into adhesive fracture toughness. Some aspects of the analsis of the elastic and plastic deformations will be seen to be similar. Laminates that can be peeled can be classified into two tpes. First, where the adhesive laer thickness is negligible e.g. two polmer films that are fused together. Second, where the adhesive laer thickness is not negligible and for which it might be necessar to accommodate the deformation within the adhesive laer during the peel bending process. Such laminates might include metal/polmer/metal sstems. This protocol will accommodate both tpes of sstem.
2 2 2 FIXED ARM PEEL TEST. 2.1 ANALYSIS OF THE FIXED ARM PEEL TEST. Peel arm (thickness h Peel force P Laminate of width b θ Peel angle Fixed arm of laminate Figure 1 Fixed arm peel test Figure 1 shows the peel of a laminate at a peel angle of θ with a force P acting on the peel arm (width b, thickness h. In order to peel one laer of the laminate from the other, it is necessar to provide energ in the form of external work to the laminate. The energ contributions to a fixed arm peel procedure can be described b a global energ analsis [1]. The input energ to the peel test needs to be resolved into the various deformational energies, elastic, plastic and adhesive fracture energies, at least. G A du ext du s du dt du db = ( 1 bda bda bda bda where G A is the adhesive fracture toughness, U is energ with subscripts ext, s, dt and db referring to external work, strain energ, dissipated tensile energ and dissipated bending energ, respectivel. b is the specimen width and da the peel fracture length. This approach has been applied to a fixed arm peel test [1, 2] in order to convert peel strength (P/b to adhesive fracture toughness: G = G ( 2 A G P G is the input energ after correction for tensile elastic and plastic deformation in the peel arm and G P is the plastic work in bending the peel arm. The tensile corrections are often negligible [1] and then input energ is given b: P G = ( 1 cosθ (3 b θ is the peel angle. In order to calculate the plastic deformation energ associated with the peel arm, it is first necessar to have knowledge of the tensile stressstrain characteristics of the peel arm material. This will include an initial elastic deformation but also a subsequent work hardening, plastic, deformation. The plastic bending in the peel tests ma then be
3 3 modelled using largedisplacement beam theor with modifications for plastic bending. Solutions have been formulated for three cases: (i Digitised, where the stressstrain behaviour of the peel arm is digitised and a numerical analsis is used to calculate G P [3]. (ii Bilinear, where a bilinear fit is given to the stressstrain curve and an analtical calculation of G P [4,5]. (iii Power law, where an linear elasticpower law plastic fit is given to the stressstrain curve and an analtical calculation of G P [4,5]. For the bilinear and power law curve fits, the details are as follows where a number of parameters from the stressstrain fits are calculated. N is a constant, α is the ratio of plastic modulus to elastic modulus i.e. E 2 /E 1, σ is ield stress and ε is ield strain. N and α are the respective work hardening coefficients for power law and linear work hardening. When ε ε, σ = Eε ( 3 in both cases, and whenε >, N ε ε σ = σ ( ( 4 ε in the power law work hardening model, and σ = σ + αe( ε ε ( 5 for the bilinear model. For laminates where the adhesive laer thickness (h A is ver small, h A 0, there is no requirement to consider the deformation in the adhesive in conducting the calculations of adhesive fracture toughness [4]. However, when h A >0 the deformation in the adhesive laer should be included in the analsis for which it will be necessar to have knowledge of the modulus of the adhesive material (E A. In all, these various calculations can be complex and whilst a theoretical analsis is given in reference [4], software (ICPeel that can be used to conduct the calculations is available on the Imperial College London website [6]. The digitisation of the stressstrain behaviour also requires a software package as does the subsequent numerical analsis for calculation of G P. This is also provided on the Imperial College London website [6] where the package is called ICPeel (Digitised. In principle, the digitised approach should be the most accurate but it is also the most cumbersome and timeconsuming approach. However, the digitised package is quite quick if an approximate solution is used first. This is based on using the stressstrain parameters form the curve fitting procedures prior to conducting an accurate analsis. Therefore, it is necessar to run ICPeel first and ICPeel (Digitised next. Consequentl, it is helpful to use the results from all three cases in the determination of G P and G A. The website includes instructions on how to run the packages. In order to determine G A without neglecting an of the elastic or plastic deformations, two experiments are required:
4 4 (a The peel test with a control of the peel angle. (b A tensile stressstrain measurement of the peel arm up to fracture or at least to a strain magnitude that exceeds the maximum strain in the peel test (this is given in ICPeel and is tpicall 6%. Experimental requirements for both of these measurements are given in section 2.2 and Straight line fitted to elastic curve True Stress (MPa Straight line fitted to initial plastic curve Interception of these lines provides the ield coordinates True Strain Figure 2 Definition of ield coordinates A critical issue in analsing these curves concerns the definition of the ield coordinates (ε, σ. These are obtained from the experimental data b fitting a straight line to the linear elastic region of the curve and a straight line to the initial plastic region of the curve, as shown in Figure 2. The straight line fitted to the initial plastic curve should start beond an approximate ield point and end at approximatel 10 times the ield strain, again as shown in Figure 2. The interception of these two lines defines the ield coordinates. The measured stressstrain curve is then modelled to either a bilinear form, as shown in Figure 3 or a power law form as shown in Figure 4. Both fits should be conducted for the purpose of calculation of G P and G A, but also for the ICPeel (Digitised analsis. The fitted curves must compl with these ield coordinates (as equations 35 indicate. Therefore, once the ield coordinates are defined from the experimental curve, then the linear elastic portion for both models is the line between the origin and these coordinates. The plastic region then starts beond the ield coordinates but for both tpes of model, the fitted curve must pass through the ield coordinates. In general, net stress (force/original cross sectional area and net strain (increase in length/gauge length are used. However, if the strain exceeds 10% then a true stress should be used (true stress = net stress [1+ strain].
5 5 250 True Stress (MPa Experimental curve E 1 E 2 Yield coordinates (ε,σ True Strain Figure 3 Tensile stress versus strain plot for a peel arm illustrating a bilinear elasticplastic fit and the definition of E 1, E 2 and ield strain 200 True Stress (MPa Experimental curve Yield coordinates (ε,σ True Strain Figure 4 An illustration of an elastic region followed b a power law fit for work hardening. Adhesive fracture toughness is determined according to equation 2. Ideall, the corrections for plastic deformation should not be too large otherwise errors for the determination of
6 6 adhesive fracture toughness will become significant. The size of this correction is given b G ( P x100% ; the smaller this correction the better [2]. G These considerations appl equall to the Tpeel analsis but can onl be determined for each peel arm separatel. 2.2 EXPERIMENTAL PROCEDURES IN THE FIXED ARM PEEL TEST. Specimens for conducting peel strength should be in the form of rectangular specimens where the two parts of the laminate have alread been adhered but where there is a region of unadhered material (of nominal length 30 mm. The overall dimensions of a peel specimen need not be rigidl defined but for man tests we have found that a length of 100 mm and width 20 mm proves to be quite satisfactor. Three specimens should be tested for each set of conditions. The choice of peel jig is not unique but the apparatus should incorporate a number of facilities. A successful kit is shown schematicall in Figure 5. First, the apparatus should be able to select the peel angle in the range up to 180. Second, the jig is attached to an Instron or similar universal testing machine such that as peel occurs the peel angle is maintained constant b the jig moving along a low friction linear bearing sstem. Third, onl one side of the laminate is allowed to be the peel arm in the test. Of course, the laminate can be reversed so changing the peel arm material in another but separate test. (Consequentl, the composition of the adherends ma or ma not be the same. Adhering one side of the laminate to the peel table is a critical issue. If this laer can separate from the table during the test then the energ involved in that process will increase the measured adhesive fracture toughness value to an erroneousl high level. The means of gluing the laer to the table should be reported. The material used for the peel arm (substrate should be reported, as should the length, width and thickness dimensions of the specimen (h and h A where h is the thickness of the substrate alone (i.e. without an coating of adhesive and h A is the thickness of the adhesive. The peel angle needs to be selected on the basis of ensuring that the peel force is large compared with the resolution of the load cell and the frictional forces in the test. For purposes of the protocol it will be necessar to conduct the test at a range of peel angles between 45 o and 135 o but the peel angle 90 o δ should alwas be one of the angles. A peel test speed ( t of 10 mm/min can be used as a standard speed with the 90 o. However, the peel angle will a influence the peel crack speed (. t δ a = (1 cos θ (6 t t Therefore, when conducting tests over a range of peel angles it us necessar to select a common peel crack speed.
7 7 Figure 5 Fixed arm peel fixture with linear bearing sstem showing a peel angle of 45 o. The force versus displacement curve to initiate and propagate a peel fracture should be recorded. At least 30 mm of peel fracture should be established. The average peel force should then be determined as shown in Figure 6A. If there is a combination of adhesive and cohesive fracture or stickslip (as illustrated in Figure 6B, then for these occasions, both the mean lowest and the mean highest stead propagation peel force values should then be used to determine the adhesive and cohesive fracture toughness values, respectivel. 400 Peel force (N Onset of peel Average peel force Displacement (mm Figure 6A: Illustrative peel force versus displacement demonstrating how to average the peel force.
8 8 2.5 Cohesive peel force Force N mm Deflection Adhesive peel force Figure 6B Peel force versus deflection in a fixed arm peel test. The higher peel forces relate to cohesive fracture; the lower peel forces relate to adhesive fracture In order to conduct the corrections summarised in equations 25 it is necessar to obtain a tensile stress  strain plot on the material of the peel arm. (This should be the substrate material alone i.e. it should not be the substrate with a coating of adhesive material. In order to accommodate current analtical methods for the determination of the plastic work in bending the peel arm, this stressstrain plot will need to be described either as a bilinear function or as a linear elasticpower law plastic function or as a digitised function. The tensile test should be conducted at the same test speed as the peel test and in order to obtain sufficient accurac the test specimen should be a rectangular strip of width 10 mm and length 100 mm. In addition, an extensometer will be required to measure the strain deformations necessar to define the elastic deformations. The extensometer, ideall, should be of a noncontacting tpe, since the peel arms are likel to be of low stiffness. The tensile test should continue in order to enable a clear definition of the plastic region of the deformations b continuing the test to fracture. The comments preceding Figure 3 provide instructions for fitting a bilinear elasticplastic fit for the stressstrain curve. Five parameters should be obtained, namel E 1, E 2, α (E 2 /E 1, ε and σ. The elastic modulus (E 1 is defined as the slope of the stressstrain curve at small deformations and before ielding has occurred. In order to define the plastic modulus (E 2 it is helpful to allow the tensile specimen to continue extension for as long as possible. If it transpires that the "work hardening" portion of the stressstrain curve exhibits a negative slope, then values of α and E 2 should be made zero (and not negative. In order to construct a linear elastic region followed b a power law work hardening region, the scheme shown in the text preceding Figure 4 should be used. The definition of the elastic region is as above and the power law fit should onl be made for post ield data. The parameters that should be obtained from the analsis are E 1, N, ε and σ. The coordinates at ield (as defined in an earlier section are given b the intercept of the elastic line and the plastic region for the experimental curve. Therefore, if the general power law gives N σ = Aε (7 The elastic region is
9 9 σ = E1ε (8 At ield, the stress (σ is σ and the strain (ε is ε. Therefore eliminating σ from equations 7 and 8 gives an expression for ield strain, 1 A 1 N = ( E1 ε (9 and ield stress is σ = E ε ( TEST REPORT FOR THE FIXED ARM PEEL TESTS The following information is required in the test report. General information Name of Laborator Description of laminate Material of peel arm Adhesive used for gluing one arm to the peel table Test equipment Data from tensile test on the peel arm material Test speed (mm/min Bilinear fit Low strain modulus (E 1 (GPa Power law fit Low strain modulus (E 1 (GPa N Yield strain (% High strain modulus (E 2 (GPa Yield strain (% Alpha (E 2 /E 1 Yield stress (MPa Yield stress (MPa Data from the peel test Peel angle ( o Test speed (mm/min Specimen dimensions L (mm b (mm Peel arm thickness h (µm (substrate onl Thickness of adhesive laer h A (µm (if h A > 0 then conduct calculations for two cases h A = 0 and the actual value for h A Value ascribed to the modulus of the adhesive E A (GPa Peel strength (P/b (N/mm Derived results b calculations (for each of the three fits to the stressstrain data G (J/m 2 G P (J/m 2
10 10 G A (J/m 2 Correction factor (% Results should be presented for each specimen. The report should include a plot of the peel curve (i.e. force versus displacement in the peel test. The length of peel growth should be marked on this curve together with a clear indication as to how the peel force used to determine the peel strength is derived from the plot. (Figure 6 shows an illustration of the requirement. In addition, the tensile stressstrain plots with the bilinear and/or power law fits should be reported 3 TPEEL TEST 3.1 ANALYSIS OF THE TPEEL TEST. Figure 7 shows the specimen configuration during a Tpeel test. When the stiffness of the peel arms is different the peel angles will be φ and θ (rather than 90 o. In Figure 7 the stiffer arm is peel arm 2, therefore φ<90 and θ>90. The analsis proceeds along similar lines to that in the fixed arm peel test (see section 2.1, except that there are now two peel arms to accommodate. However, onl one of the peel angles needs to be considered since φ = π θ: P G = (1 + cos (6 b 1 φ P G = (1 cos (7 b 2 φ Where the super scripts 1 and 2 refer to the two peel arms, respectivel. The peel toughness terms for elastic corrections are then similar to those in equation (3, except that there are two terms. In a similar manner, there will be two terms for the dissipated energ. Consequentl, there will be two forms for equations (2: G = G G (8 ( A 1 1 ( P 1 G = G G (9 ( A 2 2 ( P 2
11 11 Peel force P Peel arm Specimen of width b θ φ Peel arm 2 Figure 7: TPeel Specimen During a Test. The adhesive fracture toughness (G A from the Tpeel test is then the sum of the terms from equations (8 and (9, namel: G + A ( GA 1 ( GA 2 = ( EXPERIMENTAL PROCEDURES IN THE T PEEL TEST. Specimens for conducting peel strength should be in the form of rectangular specimens where the two parts of the laminate have alread been adhered but where there is a region of unadhered material (of nominal length 30 mm. The overall dimensions of a peel specimen need not be rigidl defined but for man tests we have found that a length of 100 mm and width 20 mm proves to be quite satisfactor. Three specimens should be tested for each set of conditions and care should be taken to ensure that no part of the peel arms can touch the test equipment. There are two configurations for conducting the Tpeel tests, as shown in Figure 8. Configuration A has the stiffer peel arm at the bottom, whilst configuration B has the stiffer peel arm at the top. It is likel that the small peel angle for these configurations will not be the same since the stiffer peel arm, which could contain more mass than the less stiff peel arm, will hang differentl. Three specimens tested in either configuration A or B should be conducted and the configuration tpe recorded.
12 12 Peel arm 1 Stiffer arm Peel arm 2 Configuration A Configuration B Figure 8 Specimen configurations for Tpeel The materials of the peel arms ma or ma not be the same. The test machine should have the usual capabilities for sufficient resolution of force. Once the peel arms are in tension, the specimen configuration will be similar to one of those shown in Figure 8. During the course of peeling it is necessar to measure one of the peel angles (φ or ϕ and at least three measurements should be made throughout the 30 mm peel fracture; one near the start, one in the middle and one near the end. The average value for the peel angle can then be determined and used in the calculations. A peel test speed of 10 mm/min can be used as a standard. However, if there are large variations in measured peel angle (e.g. > 30 o between specimens or samples then equation 6 should be used to adjust to a common crack speed. (This will be a retrospective judgement. The force versus displacement curve to initiate and propagate a peel fracture should be recorded. At least 30 mm of peel fracture should be established. The average peel force should then be determined unless there is a combination of adhesive and cohesive fracture or stickslip (as illustrated in Figure 6. For these occasions, the mean lowest and the mean highest stead propagation peel force values should then be used to determine the adhesive and the cohesive fracture toughness values, respectivel. In order to conduct the corrections summarised in equations 610, it is necessar to measure tensile stress  strain plots on the material of the peel arms. (Two tensile stressstrain plots will be required if the materials of the peel arms are different. Establishing digitised, bilinear and elasticpower law plastic descriptions of the tensile stressstrain behaviour of the peel arms should be done as previousl described in the section on fixed arm tests. Calculation of the various adhesive fracture toughness terms is then done for each peel arm as described in the section on the fixed arm peel. 3.3 TEST REPORT FOR THE TPEEL TESTS The information required in a test report is similar to that for the fixed arm test. However, for the Tpeel test there will be two peel arms to report and two possible specimen configurations (A and B as well as the measured peel angle. However, there is no requirement to test both tpes of configuration. The information required is as follows:
13 13 General information Name of Laborator Description of laminate Material of peel arm Adhesive used for gluing one arm to the peel table Test equipment Data from tensile test(s on the peel arm material(s This should be provided for both peel arms (1 and 2 if different. Test speed (mm/min Bilinear fit Power law fit Low strain modulus (E 1 (GPa Low strain modulus (E 1 (GPa Yield strain (% N High strain modulus (E 2 (GPa Yield strain (% Alpha (E 2 /E 1 Yield stress (MPa Yield stress (MPa Data from the peel test Specimen configuration (A or B Measured peel angle ( o [The smaller angle should be quoted] Test speed (mm/min Specimen dimensions L (mm b (mm Peel arm thickness h (µm (substrate onl Thickness of adhesive laer h A (µm (if h A > 0 then conduct calculations for two cases h A = 0 and the actual value for h A Value ascribed to the modulus of the adhesive E A (GPa Peel strength (P/b (N/mm Derived results b calculations (for each of the three fits to the stressstrain data To be quoted for each peel arm G (J/m 2 G P (J/m 2 G A (J/m 2 Correction factor (% Overall results G A =(G A 1 +(G A 2 CONCLUDING COMMENTS It would be helpful to use both test methods in order to determine the adhesive fracture toughness. Provided that the correction factor is not too large, then it can be hoped that the values will be the same for both test methods. It is recommended that the software source used for the calculations is quoted in all reports.
14 14 REFERENCES 1 Kinloch, A.J., Lau, C.C. and J G Williams, Int. J. Fract., 66, ( Moore, D.R., Williams, J.G., Fracture of Polmers, Composites and Adhesives, ESIS pub 32, ISBN: , Elsevier, L. F. Kawashita The Peeling of Adhesive Joints PhD thesis Universit of London Georgiou, I., Hadavina, H., Ivankovic, A., Kinloch, A.J., Tropsa, V., Williams, J. G., The Journal of Adhesion, 79, 127 ( Lau, C. C., PhD Thesis, Universit of London ( Imperial College London Website,
Using ABAQUS Cohesive Elements to Model Peeling of an Epoxybonded Aluminum Strip: A Benchmark Study for Inelastic Peel Arms
Using ABAQUS Cohesive Elements to Model Peeling of an Epoxybonded Aluminum Strip: A Benchmark Study for Inelastic Peel Arms Ted Diehl DuPont DuPont Engineering Technology, Chestnut Run, Bldg 722, Wilmington,
More informationA SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST
A SELFINDICATING MODE I INTERLAMINAR TOUGHNESS TEST P. Robinson The Composites Centre, Department of Aeronautics, Imperial College London South Kensington, London, SW7 2AZ, UK p.robinson@imperial.ac.uk
More informationA Direct Derivation of the GriffithIrwin Relationship using a Crack tip Unloading Stress Wave Model.
A Direct Derivation of the GriffithIrwin Relationship using a Crack tip Unloading Stress Wave Model. C.E. NealSturgess. Emeritus Professor of Mechanical Engineering, The Universit of Birmingham, UK.
More informationFigure 1. Simplysupported beam nomenclature with single point load. Typical shear and moment diagrams are also shown.
CE0L Student Lab Manual Wood Flexural Strength Introduction This section outlines the steps necessar to perform the Wood Flexural Strength lab experiment. The purpose of the lab is to determine the Modulus
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 3
MECE 3321 MECHANICS OF SOLIDS CHAPTER 3 Samantha Ramirez TENSION AND COMPRESSION TESTS Tension and compression tests are used primarily to determine the relationship between σ avg and ε avg in any material.
More informationLaboratory 4 Bending Test of Materials
Department of Materials and Metallurgical Engineering Bangladesh University of Engineering Technology, Dhaka MME 222 Materials Testing Sessional.50 Credits Laboratory 4 Bending Test of Materials. Objective
More informationStressStrain Behavior
StressStrain Behavior 6.3 A specimen of aluminum having a rectangular cross section 10 mm 1.7 mm (0.4 in. 0.5 in.) is pulled in tension with 35,500 N (8000 lb f ) force, producing only elastic deformation.
More informationOutline. TensileTest Specimen and Machine. StressStrain Curve. Review of Mechanical Properties. Mechanical Behaviour
TensileTest Specimen and Machine Review of Mechanical Properties Outline Tensile test True stress  true strain (flow curve) mechanical properties:  Resilience  Ductility  Toughness  Hardness A standard
More informationIntroduction to Engineering Materials ENGR2000. Dr. Coates
Introduction to Engineering Materials ENGR2 Chapter 6: Mechanical Properties of Metals Dr. Coates 6.2 Concepts of Stress and Strain tension compression shear torsion Tension Tests The specimen is deformed
More informationSimulation of Nonlinear Behavior of WallFrame Structure during Earthquakes
Simulation of Nonlinear Behavior of WallFrame Structure during Earthquakes b Masaomi Teshigawara 1, Hiroshi Fukuama 2, Hiroto Kato 2, Taiki Saito 2, Koichi Kusunoki 2, Tomohisa Mukai 2 ABSTRACT The reinforced
More informationFREE EDGE DELAMINATION ONSET CRITERION
FREE EGE ELAMINATION ONSET CRITERION G. MARION now, 2, formerl 3, R. HARRY 2, and F. LECUYER MEYSYS, 29 rue J. Rostand, 9873 ORSAY CEEX, FRANCE 2 Laboratoire de Génie Mécanique, IUT Bordeaux I, 3345 TALENCE
More information1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine Spring 2004 LABORATORY ASSIGNMENT NUMBER 6
1.103 CIVIL ENGINEERING MATERIALS LABORATORY (123) Dr. J.T. Germaine MIT Spring 2004 LABORATORY ASSIGNMENT NUMBER 6 COMPRESSION TESTING AND ANISOTROPY OF WOOD Purpose: Reading: During this laboratory
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 4 Pure Bending
EA 3702 echanics & aterials Science (echanics of aterials) Chapter 4 Pure Bending Pure Bending Ch 2 Aial Loading & Parallel Loading: uniform normal stress and shearing stress distribution Ch 3 Torsion:
More informationNCHRP FY 2004 Rotational Limits for Elastomeric Bearings. Final Report APPENDIX E. John F. Stanton Charles W. Roeder Peter MackenzieHelnwein
NCHRP 68 FY 4 Rotational Limits for Elastomeric Bearings Final Report APPENDIX E John F. Stanton Charles W. Roeder Peter MackenzieHelnwein Department of Civil and Environmental Engineering Universit
More informationPhysical Properties Testing Technical Bulletin
Technical Bulletin MANUFACTURER Raven Lining Systems 13105 E. 61 st Street, Suite A Broken Arrow, OK 74012 (918) 6150020 TENSILE TESTING OF PLASTICS ASTM D638, ISO 527 Tensile tests measure the force
More informationA CompressionLoaded Double Lap Shear Test: Part 1, Theory
International Journal of Adhesion and Adhesives, submitted A CompressionLoaded Double Lap Shear Test: Part 1, Theor D.A. Mendels, S.A. Page, J.A. E. Månson Laboratoire de Technologie des Composites
More informationIntroduction to Fracture
Introduction to Fracture Introduction Design of a component Yielding Strength Deflection Stiffness Buckling critical load Fatigue Stress and Strain based Vibration Resonance Impact High strain rates Fracture
More informationExperimental Uncertainty Review. Abstract. References. Measurement Uncertainties and Uncertainty Propagation
Experimental Uncertaint Review Abstract This is intended as a brief summar of the basic elements of uncertaint analsis, and a hand reference for laborator use. It provides some elementar "rulesofthumb"
More informationChapter 7. Highlights:
Chapter 7 Highlights: 1. Understand the basic concepts of engineering stress and strain, yield strength, tensile strength, Young's(elastic) modulus, ductility, toughness, resilience, true stress and true
More informationMassachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139
Massachusetts Institute of Technology Department of Mechanical Engineering Cambridge, MA 02139 2.002 Mechanics and Materials II Spring 2004 Laboratory Module No. 6 Fracture Toughness Testing and Residual
More informationINTERFACE SHEAR TRANSFER FOR HIGH STRENGTH CONCRETE AND HIGH STRENGTH REINFORCEMENT
INTERFACE SHEAR TRANSFER FOR HIGH STRENGTH CONCRETE AND HIGH STRENGTH REINFORCEMENT 641 Susumu KONO 1 And Hitoshi TANAKA SUMMARY The shear transfer at construction joints for members with high strength
More informationDESIGN OF BEAMCOLUMNS  II
DESIGN OF BEACOLUNSII 14 DESIGN OF BEACOLUNS  II 1.0 INTRODUCTION Beamcolumns are members subjected to combined bending and axial compression. Their behaviour under uniaxial bending, biaxial bending
More informationA CRITERION OF TENSILE FAILURE FOR HYPERELASTIC MATERIALS AND ITS APPLICATION TO VISCOELASTICVISCOPLASTIC MATERIALS
MTS ADHESIVES PROGRAMME 19961999 PERFORMANCE OF ADHESIVE JOINTS Project: PAJ1; Failure Criteria and their Application to ViscoElastic/ViscoPlastic Materials Report 2 A CRITERION OF TENSILE FAILURE FOR
More informationChapter 5: Ball Grid Array (BGA)
Chapter 5: Ball Grid Array (BGA) 5.1 Development of the Models The following sequence of pictures explains schematically how the FEmodel of the Ball Grid Array (BGA) was developed. Initially a single
More information6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa ( psi) and
6.4 A cylindrical specimen of a titanium alloy having an elastic modulus of 107 GPa (15.5 10 6 psi) and an original diameter of 3.8 mm (0.15 in.) will experience only elastic deformation when a tensile
More information4.MECHANICAL PROPERTIES OF MATERIALS
4.MECHANICAL PROPERTIES OF MATERIALS The diagram representing the relation between stress and strain in a given material is an important characteristic of the material. To obtain the stressstrain diagram
More informationNigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37
Nigerian Journal of Technology, Vol. 26, No. 2, June 2007 Edelugo 37 APPLICATION OF THE REISSNERS PLATE THEORY IN THE DELAMINATION ANALYSIS OF A THREEDIMENSIONAL, TIME DEPENDENT, NONLINEAR, UNIDIRECTIONAL
More informationEXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES
20 th International Conference on Composite Materials Copenhagen, 1924 th July 2015 EXPERIMENTAL CHARACTERIZATION AND COHESIVE LAWS FOR DELAMINATION OF OFFAXIS GFRP LAMINATES Esben Lindgaard 1 and Brian
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More information3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture,
3.032 Problem Set 2 Solutions Fall 2007 Due: Start of Lecture, 09.21.07 1. In the beam considered in PS1, steel beams carried the distributed weight of the rooms above. To reduce stress on the beam, it
More informationMODELING OF NONLINEAR BEHAVIOR OF RC SHEAR WALLS UNDER COMBINED AXIAL, SHEAR AND FLEXURAL LOADING
CD02003 MODELING OF NONLINEAR BEHAVIOR OF RC SHEAR WALLS UNDER COMBINED AXIAL, SHEAR AND FLEXURAL LOADING B. Ghiassi 1, M. Soltani 2, A. A. Tasnimi 3 1 M.Sc. Student, School of Engineering, Tarbiat Modares
More informationDelamination in fractured laminated glass
Delamination in fractured laminated glass Caroline BUTCHART*, Mauro OVEREND a * Department of Engineering, University of Cambridge Trumpington Street, Cambridge, CB2 1PZ, UK cvb25@cam.ac.uk a Department
More informationSeismic Pushover Analysis Using AASHTO Guide Specifications for LRFD Seismic Bridge Design
Seismic Pushover Analysis Using AASHTO Guide Specifications for LRFD Seismic Bridge Design Elmer E. Marx, Alaska Department of Transportation and Public Facilities Michael Keever, California Department
More informationASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE MATERIAL
5 th International Conference Advanced Composite Materials Engineering COMAT 2014 1617 October 2014, Braşov, Romania ASPECTS CONCERNING TO THE MECHANICAL PROPERTIES OF THE GLASS / FLAX / EPOXY COMPOSITE
More informationEnergy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing the effect of residual stresses
International Journal of Adhesion & Adhesives 20 (1999) 59 70 International Journal of Adhesion & Adhesives Energy release rate analysis for adhesive and laminate double cantilever beam specimens emphasizing
More informationPacific Earthquake Engineering Research Center
Pacific Earthquake Engineering Research Center Performance Models for Flexural Damage in Reinforced Concrete Columns Michael Berr and Marc Eberhard Department of Civil & Environmental Engineering Universit
More informationFRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING.
FRACTURE TOUGHNESS OF ADHESIVE BONDED COMPOSITE JOINTS UNDER MIXED MODE LOADING. X. J. Gong, F. Hernandez, G. Verchery. ISAT  Institut Supérieur de l Automobile et des Transports, LRMA  Laboratoire de
More informationσ = Eα(T T C PROBLEM #1.1 (4 + 4 points, no partial credit)
PROBLEM #1.1 (4 + 4 points, no partial credit A thermal switch consists of a copper bar which under elevation of temperature closes a gap and closes an electrical circuit. The copper bar possesses a length
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationUK, tel ; 2 EDF Energy, Barnett Way, Barnwood, Gloucester, GL4 3RS,
The RatchetShakedown Diagram for a Thin Pressurised Pipe Subject to Additional Axial Load and Cclic Secondar Global Bending R.A.W.Bradford and D.J.Tipping Universit of Bristol, Mechanical Engineering,
More informationPullout Tests of Geogrids Embedded in Noncohesive Soil
Archives of HydroEngineering and Environmental Mechanics Vol. 51 (2004), No. 2, pp. 135 147 Pullout Tests of Geogrids Embedded in Noncohesive Soil Angelika Duszyńska, Adam F. Bolt Gdansk University of
More informationTHE GENERAL ELASTICITY PROBLEM IN SOLIDS
Chapter 10 TH GNRAL LASTICITY PROBLM IN SOLIDS In Chapters 35 and 89, we have developed equilibrium, kinematic and constitutive equations for a general threedimensional elastic deformable solid bod.
More informationMechanical properties 1 Elastic behaviour of materials
MME131: Lecture 13 Mechanical properties 1 Elastic behaviour of materials A. K. M. B. Rashid Professor, Department of MME BUET, Dhaka Today s Topics Deformation of material under the action of a mechanical
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationFATIGUE ANALYSIS: THE SUPERNEUBER TECHNIQUE FOR CORRECTION OF LINEAR ELASTIC FE RESULTS
6 TH INTERNATIONAL CONGRESS OF THE AERONAUTICAL SCIENCES FATIGUE ANALYSIS: THE SUPERNEUBER TECHNIQUE FOR CORRECTION OF LINEAR ELASTIC FE RESULTS L. Samuelsson * * Volvo Aero Corporation, Sweden Kewords:
More informationElasticPlastic Fracture Mechanics. Professor S. Suresh
ElasticPlastic Fracture Mechanics Professor S. Suresh Elastic Plastic Fracture Previously, we have analyzed problems in which the plastic zone was small compared to the specimen dimensions (small scale
More information7.4 The Elementary Beam Theory
7.4 The Elementary Beam Theory In this section, problems involving long and slender beams are addressed. s with pressure vessels, the geometry of the beam, and the specific type of loading which will be
More informationVibrational Power Flow Considerations Arising From MultiDimensional Isolators. Abstract
Vibrational Power Flow Considerations Arising From MultiDimensional Isolators Rajendra Singh and Seungbo Kim The Ohio State Universit Columbus, OH 4321117, USA Abstract Much of the vibration isolation
More informationDeflections and Strains in Cracked Shafts Due to Rotating Loads: A Numerical and Experimental Analysis
International Journal of Rotating Machinery, 9: 303 311, 2003 Copyright c Taylor & Francis Inc. ISSN: 1023621X DOI: 10.1080/10236210390147416 Deflections and Strains in Cracked Shafts Due to Rotating
More informationDeflections and Strains in Cracked Shafts due to Rotating Loads: A Numerical and Experimental Analysis
Rotating Machinery, 10(4): 283 291, 2004 Copyright c Taylor & Francis Inc. ISSN: 1023621X print / 15423034 online DOI: 10.1080/10236210490447728 Deflections and Strains in Cracked Shafts due to Rotating
More informationInitial Stress Calculations
Initial Stress Calculations The following are the initial hand stress calculations conducted during the early stages of the design process. Therefore, some of the material properties as well as dimensions
More informationTHEME IS FIRST OCCURANCE OF YIELDING THE LIMIT?
CIE309 : PLASTICITY THEME IS FIRST OCCURANCE OF YIELDING THE LIMIT? M M  N N + + σ = σ = + f f BENDING EXTENSION Ir J.W. Welleman page nr 0 kn Normal conditions during the life time WHAT HAPPENS DUE TO
More informationFCP Short Course. Ductile and Brittle Fracture. Stephen D. Downing. Mechanical Science and Engineering
FCP Short Course Ductile and Brittle Fracture Stephen D. Downing Mechanical Science and Engineering 001015 University of Illinois Board of Trustees, All Rights Reserved Agenda Limit theorems Plane Stress
More informationOPTIMISING THE MECHANICAL CHARACTERISATION OF A RESILIENT INTERLAYER FOR THE USE IN TIMBER CON STRUCTION
OPTIMISING THE MECHANICAL CHARACTERISATION OF A RESILIENT INTERLAYER FOR THE USE IN TIMBER CON STRUCTION Luca Barbaresi, Federica Morandi, Juri Belcari, Andrea Zucchelli and Alice Speranza University
More informationMAE 323: Chapter 4. Plane Stress and Plane Strain. The Stress Equilibrium Equation
The Stress Equilibrium Equation As we mentioned in Chapter 2, using the Galerkin formulation and a choice of shape functions, we can derive a discretized form of most differential equations. In Structural
More informationChapter 12. Static Equilibrium and Elasticity
Chapter 12 Static Equilibrium and Elasticity Static Equilibrium Equilibrium implies that the object moves with both constant velocity and constant angular velocity relative to an observer in an inertial
More informationFigure 1. Dimension of PSA in face paper laminate
EVALUATION OF DYNAMIC MECHANICAL PROPERTIES OF PRESSURE SENSITIVE ADHESIVE IN PAPER LANIMATES FOR POSTAGE STAMP APPLICATION: METHOD DEVELOPMENT AND ADHESIVE CHARACTERIZATION Hailing Yang, Graduate Student,
More informationAfter lecture 16 you should be able to
Lecture 16: Design of paper and board packaging Advanced concepts: FEM, Fracture Mechanics After lecture 16 you should be able to describe the finite element method and its use for paper based industry
More informationEffect of Strain Hardening on Unloading of a Deformable Sphere Loaded against a Rigid Flat A Finite Element Study
Effect of Strain Hardening on Unloading of a Deformable Sphere Loaded against a Rigid Flat A Finite Element Study Biplab Chatterjee, Prasanta Sahoo 1 Department of Mechanical Engineering, Jadavpur University
More informationTHE DETERMINATION OF FRACTURE STRENGTH FROM ULTIMATE TENSILE AND TRANSVERSE RUPTURE STRESSES
Powder Metallurgy Progress, Vol.3 (003), No 3 119 THE DETERMINATION OF FRACTURE STRENGTH FROM ULTIMATE TENSILE AND TRANSVERSE RUPTURE STRESSES A.S. Wronski, A.Cias Abstract It is wellrecognized that the
More informationPLASTIC FLOW THROUGHOUT VOLUME OF THIN ADHESIVE!BONDS. No March 1958 (.2. Will In' iriculture ROOM. Mum mina
iriculture ROOM (.2 PLASTIC FLOW THROUGHOUT VOLUME OF THIN ADHESIVE!BONDS No. 2092 March 1958 11 Will In' Mum mina FOREST PRODUCTS LABORATORY MADISON 5, WISCONSIN UNITED STATES DEPARTMENT OF AGRICULTURE
More informationEVALUATION OF THERMAL TRANSPORT PROPERTIES USING A MICROCRACKING MODEL FOR WOVEN COMPOSITE LAMINATES
EVALUATION OF THERMAL TRANSPORT PROPERTIES USING A MICROCRACKING MODEL FOR WOVEN COMPOSITE LAMINATES C. Luo and P. E. DesJardin* Department of Mechanical and Aerospace Engineering Universit at Buffalo,
More informationMaterials: engineering, science, processing and design, 2nd edition Copyright (c)2010 Michael Ashby, Hugh Shercliff, David Cebon.
Modes of Loading (1) tension (a) (2) compression (b) (3) bending (c) (4) torsion (d) and combinations of them (e) Figure 4.2 1 Standard Solution to Elastic Problems Three common modes of loading: (a) tie
More informationStrain Transformation and Rosette Gage Theory
Strain Transformation and Rosette Gage Theor It is often desired to measure the full state of strain on the surface of a part, that is to measure not onl the two etensional strains, and, but also the shear
More informationBasic principles of steel structures. Dr. Xianzhong ZHAO
Basic principles of steel structures Dr. Xianzhong ZHAO.zhao@mail.tongji.edu.cn www.sals.org.cn 1 Introduction Resistance of crosssection Compression members Outlines Overall stabilit of uniform (solid
More informationFRACTURE MECHANICS FOR MEMBRANES
FRACTURE MECHANICS FOR MEMBRANES Chong Li, Rogelio Espinosa and Per Ståhle Solid Mechanics, Malmö University SE 205 06 Malmö, Sweden chong.li@ts.mah.se Abstract During fracture of membranes loading often
More informationTensile behaviour of antisymmetric CFRP composite
Available online at www.sciencedirect.com Procedia Engineering 1 (211) 1865 187 ICM11 Tensile behaviour of antisymmetric CFRP composite K. J. Wong a,b, *, X. J. Gong a, S. Aivazzadeh a, M. N. Tamin b
More informationProf. Dr. Zahid Ahmad Siddiqi BEAM COLUMNS
BEA COLUNS Beam columns are structural members that are subjected to a combination of bending and axial stresses. The structural behaviour resembles simultaneousl to that of a beam and a column. ajorit
More informationMARKS DISTRIBUTION AS PER CHAPTER (QUESTION ASKED IN GTU EXAM) Name Of Chapter. Applications of. Friction. Centroid & Moment.
Introduction Fundamentals of statics Applications of fundamentals of statics Friction Centroid & Moment of inertia Simple Stresses & Strain Stresses in Beam Torsion Principle Stresses DEPARTMENT OF CIVIL
More informationAnálisis Computacional del Comportamiento de Falla de Hormigón Reforzado con Fibras Metálicas
San Miguel de Tucuman, Argentina September 14 th, 2011 Seminary on Análisis Computacional del Comportamiento de Falla de Hormigón Reforzado con Fibras Metálicas Antonio Caggiano 1, Guillermo Etse 2, Enzo
More informationACET 406 MidTerm Exam B
ACET 406 MidTerm Exam B SUBJECT: ACET 406, INSTRUCTOR: Dr Antonis Michael, DATE: 24/11/09 INSTRUCTIONS You are required to answer all of the following questions within the specified time (90 minutes).you
More information3. BEAMS: STRAIN, STRESS, DEFLECTIONS
3. BEAMS: STRAIN, STRESS, DEFLECTIONS The beam, or flexural member, is frequently encountered in structures and machines, and its elementary stress analysis constitutes one of the more interesting facets
More informationH. Hadavinia K. Nikbin Mechanical Engineering Department, Imperial College London, South Kensington Campus, United Kingdom
The Journal of Adhesion, Vol. 81, No. 5: pp 529 553, 2005 Copyright # Taylor & Francis Inc. ISSN: 00218464 print=15455823 online DOI: 10.1080/00218460590944963 Comparison of Analytical, Numerical, and
More informationCHAPTER 3 THE EFFECTS OF FORCES ON MATERIALS
CHAPTER THE EFFECTS OF FORCES ON MATERIALS EXERCISE 1, Page 50 1. A rectangular bar having a crosssectional area of 80 mm has a tensile force of 0 kn applied to it. Determine the stress in the bar. Stress
More informationSpherical Pressure Vessels
Spherical Pressure Vessels Pressure vessels are closed structures containing liquids or gases under essure. Examples include tanks, pipes, essurized cabins, etc. Shell structures : When essure vessels
More informationFracture Mechanics of NonShear Reinforced R/C Beams
Irina Kerelezova Thomas Hansen M. P. Nielsen Fracture Mechanics of NonShear Reinforced R/C Beams DANMARKS TEKNISKE UNIVERSITET Report BYG DTU R154 27 ISSN 1612917 ISBN 9788778772265 Fracture Mechanics
More informationExperiment Two (2) Torsional testing of Circular Shafts
Experiment Two (2) Torsional testing of Circular Shafts Introduction: Torsion occurs when any shaft is subjected to a torque. This is true whether the shaft is rotating (such as drive shafts on engines,
More informationMoment Area Method. 1) Read
Moment Area Method Lesson Objectives: 1) Identify the formulation and sign conventions associated with the Moment Area method. 2) Derive the Moment Area method theorems using mechanics and mathematics.
More informationX has a higher value of the Young modulus. Y has a lower maximum tensile stress than X
Bulk Properties of Solids Old Exam Questions Q1. The diagram shows how the stress varies with strain for metal specimens X and Y which are different. Both specimens were stretched until they broke. Which
More informationEE C245 ME C218 Introduction to MEMS Design
EE C245 ME C218 Introduction to MEMS Design Fall 2007 Prof. Clark T.C. Nguyen Dept. of Electrical Engineering & Computer Sciences University of California at Berkeley Berkeley, CA 94720 Lecture 16: Energy
More informationDynamic shear stress in a double lap bonded assembly
Computational Methods and Experiments in Materials Characterisation IV 167 Dynamic shear stress in a double lap bonded assembly G. Challita 1,3, R. Othman 1, P. Guegan 1, K. Khalil 2 & A. Poitou 1 1 Institut
More informationCOMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS. Abstract. Introduction
COMPRESSION AND BENDING STIFFNESS OF FIBERREINFORCED ELASTOMERIC BEARINGS HsiangChuan Tsai, National Taiwan University of Science and Technology, Taipei, Taiwan James M. Kelly, University of California,
More informationBilinear Quadrilateral (Q4): CQUAD4 in GENESIS
Bilinear Quadrilateral (Q4): CQUAD4 in GENESIS The Q4 element has four nodes and eight nodal dof. The shape can be any quadrilateral; we ll concentrate on a rectangle now. The displacement field in terms
More informationREVIEW FOR EXAM II. Dr. Ibrahim A. Assakkaf SPRING 2002
REVIEW FOR EXM II. J. Clark School of Engineering Department of Civil and Environmental Engineering b Dr. Ibrahim. ssakkaf SPRING 00 ENES 0 Mechanics of Materials Department of Civil and Environmental
More informationCHAPTER 7 EARTHQUAKE RESPONSE OF INELASTIC SYSTEMS. Base shear force in a linearly elastic system due to ground excitation is Vb
CHAPTER 7 EARTHQUAKE RESPONSE OF INELASTIC SYSTEMS Base shear force in a linearl elastic sstem due to ground excitation is Vb = ( A/ g) w where A is the pseudoacceleration corresponding to natural period
More informationDesign of a fastener based on negative Poisson's ratio foam adapted from
1 Design of a fastener based on negative Poisson's ratio foam adapted from Choi, J. B. and Lakes, R. S., "Design of a fastener based on negative Poisson's ratio foam", Cellular Polymers, 10, 205212 (1991).
More informationFlexure: Behavior and Nominal Strength of Beam Sections
4 5000 4000 (increased d ) (increased f (increased A s or f y ) c or b) Flexure: Behavior and Nominal Strength of Beam Sections Moment (kipin.) 3000 2000 1000 0 0 (basic) (A s 0.5A s ) 0.0005 0.001 0.0015
More informationtorsion equations for lateral BucKling ns trahair research report r964 July 2016 issn school of civil engineering
TORSION EQUATIONS FOR ATERA BUCKING NS TRAHAIR RESEARCH REPORT R96 Jul 6 ISSN 878 SCHOO OF CIVI ENGINEERING SCHOO OF CIVI ENGINEERING TORSION EQUATIONS FOR ATERA BUCKING RESEARCH REPORT R96 NS TRAHAIR
More informationDesign Beam Flexural Reinforcement
COPUTERS AND STRUCTURES, INC., BERKELEY, CALIFORNIA DECEBER 2001 CONCRETE FRAE DESIGN ACI31899 Technical Note This Technical Note describes how this program completes beam design when the ACI 31899
More informationFinite element modelling of infinitely wide Angleply FRP. laminates
www.ijaser.com 2012 by the authors Licensee IJASER Under Creative Commons License 3.0 editorial@ijaser.com Research article ISSN 2277 9442 Finite element modelling of infinitely wide Angleply FRP laminates
More information2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at A and supported at B by rod (1). What is the axial force in rod (1)?
IDE 110 S08 Test 1 Name: 1. Determine the internal axial forces in segments (1), (2) and (3). (a) N 1 = kn (b) N 2 = kn (c) N 3 = kn 2. Rigid bar ABC supports a weight of W = 50 kn. Bar ABC is pinned at
More informationDetermination of sizeindependent specific fracture energy of concrete from threepoint bend and wedge splitting tests
Magazine of Concrete Research, 3, 55, No. 2, April, 133 141 Determination of sizeindependent specific fracture energy of concrete from threepoint bend and wedge splitting tests H. M. Abdalla and B. L.
More informationRigid and Braced Frames
RH 331 Note Set 12.1 F2014abn Rigid and raced Frames Notation: E = modulus of elasticit or Young s modulus F = force component in the direction F = force component in the direction FD = free bod diagram
More informationMicromechanics of recycled composites
Monday, 21 st August 2011 Micromechanics of recycled composites for material optimisation and ecodesign Soraia Pimenta soraia.pimenta07@imperial.ac.uk S T Pinho, P Robinson Motivation Introduction recycled
More informationBrittle Deformation. Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm
Lecture 6 Brittle Deformation Earth Structure (2 nd Edition), 2004 W.W. Norton & Co, New York Slide show by Ben van der Pluijm WW Norton, unless noted otherwise Brittle deformation EarthStructure (2 nd
More informationAPPLIED MECHANICS I Resultant of Concurrent Forces Consider a body acted upon by coplanar forces as shown in Fig 1.1(a).
PPLIED MECHNICS I 1. Introduction to Mechanics Mechanics is a science that describes and predicts the conditions of rest or motion of bodies under the action of forces. It is divided into three parts 1.
More informationMECHANICS OF MATERIALS
Third E CHAPTER 2 Stress MECHANICS OF MATERIALS Ferdinand P. Beer E. Russell Johnston, Jr. John T. DeWolf Lecture Notes: J. Walt Oler Texas Tech University and Strain Axial Loading Contents Stress & Strain:
More informationThe fracture behaviour of structural adhesives under high rates of testing.
Engineering Fracture Mechanics, vol 76, 009, 868889 The fracture behaviour of structural adhesives under high rates of testing. B.R.K. Blackman, A.J. Kinloch, F.S. Rodriguez Sanchez, W.S. Teo & J.G. Williams
More informationIntensity (a.u.) Intensity (a.u.) Raman Shift (cm 1 ) Oxygen plasma. 6 cm. 9 cm. 1mm. Singlelayer graphene sheet. 10mm. 14 cm
Intensity (a.u.) Intensity (a.u.) a Oxygen plasma b 6 cm 1mm 10mm Singlelayer graphene sheet 14 cm 9 cm Flipped Si/SiO 2 Patterned chip Plasmacleaned glass slides c d After 1 sec normal Oxygen plasma
More informationVORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS
The 4 th World Conference on Earthquake Engineering October 7, 008, Beijing, China VORONOI APPLIED ELEMENT METHOD FOR STRUCTURAL ANALYSIS: THEORY AND APPLICATION FOR LINEAR AND NONLINEAR MATERIALS K.
More information